#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/43/4104365.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4104365
loop_
_publ_author_name
'Jamie L. Manson'
'John A. Schlueter'
'Kylee A. Funk'
'Heather I. Southerland'
'Brendan Twamley'
'Tom Lancaster'
'Stephen J. Blundell'
'Peter J. Baker'
'Francis L. Pratt'
'John Singleton'
'Ross D. McDonald'
'Paul A. Goddard'
'Pinaki Sengupta'
'Cristain D. Batista'
'Letan Ding'
'Changhoon Lee'
'Myung-Hwan Whangbo'
'Isabel Franke'
'Susan Cox'
'Chris Baines'
'Derek Trial'
_publ_contact_author_address
;
Department of Chemistry and Biochemistry
Eastern Washington University
Cheney, WA 99004
USA
;
_publ_contact_author_email       JManson@ewu.edu
_publ_contact_author_fax         '(509) 359-6973'
_publ_contact_author_name        'Dr. Jamie L. Manson'
_publ_contact_author_phone       '(509) 359-2878'
_publ_section_title
;
 Strong H...F Hydrogen Bonds as Synthons in Polymeric Quantum Magnets:
 Structural, Magnetic, and Theoretical Characterization of
 [Cu(HF₂)(pyrazine)₂]SbF₆, [Cu₂F(HF)HF₂(pyrazine)₄](SbF₆)₂
 and [CuAg(H₃F₄)(pyrazine)₅](SbF₆)₂
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              6733
_journal_page_last               6747
_journal_paper_doi               10.1021/ja808761d
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'C16 H18 Cu2 F4 N8 2+, 2(F6 Sb 1-)'
_chemical_formula_sum            'C16 H18 Cu2 F16 N8 Sb2'
_chemical_formula_weight         996.96
_chemical_name_common            '[(pyz)4Cu2(HF)F(F2H)][SbF6]2'
_space_group_IT_number           64
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           'manual editing of SHELXL-97 cif file'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   13.5893(15)
_cell_length_b                   19.974(3)
_cell_length_c                   19.893(3)
_cell_measurement_reflns_used    1847
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      28.220
_cell_measurement_theta_min      3.558
_cell_volume                     5399.6(13)
_computing_cell_refinement       'SAINT (Bruker, 2001)'
_computing_data_collection       'SMART (Siemens, 1995)'
_computing_data_reduction        'SAINT (Bruker, 2001)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2001)'
_computing_publication_material
;
SHELXTL (Sheldrick, 2001), PLATON (Spek, 2004)
;
_computing_structure_refinement  'SHELXTL (Sheldrick, 2001)'
_computing_structure_solution    'SHELXTL (Sheldrick, 2001)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Siemens SMART CCD area detector'
_diffrn_measurement_method       'area detector ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0342
_diffrn_reflns_av_sigmaI/netI    0.0191
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            20583
_diffrn_reflns_theta_full        25.24
_diffrn_reflns_theta_max         25.24
_diffrn_reflns_theta_min         2.04
_diffrn_standards_decay_%        0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.671
_exptl_absorpt_correction_T_max  0.316
_exptl_absorpt_correction_T_min  0.154
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details
;
(Sheldrick, 2001)
;
_exptl_crystal_colour            'blue grey'
_exptl_crystal_density_diffrn    2.453
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3792
_exptl_crystal_size_max          0.60
_exptl_crystal_size_mid          0.48
_exptl_crystal_size_min          0.44
_refine_diff_density_max         0.640
_refine_diff_density_min         -0.531
_refine_diff_density_rms         0.097
_refine_ls_extinction_coef       0.00056(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.079
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         2561
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.079
_refine_ls_R_factor_all          0.0244
_refine_ls_R_factor_gt           0.0233
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0343P)²+25.2831P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0710
_refine_ls_wR_factor_ref         0.0719
_reflns_number_gt                2421
_reflns_number_total             2561
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja808761d_si_006.cif
_cod_data_source_block           1b90K
_cod_original_cell_volume        5399.6(11)
_cod_original_sg_symbol_Hall     '-C 2bc 2'
_cod_database_code               4104365
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1, z+1/2'
'-x+1/2, y+1, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y-1/2, -z-1/2'
'x, -y-1/2, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y, -z-1/2'
'x+1/2, -y, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu 0.24938(4) 0.5000 0.0000 0.01444(15) Uani 1 2 d S
F1 F 0.3897(2) 0.5000 0.0000 0.0274(6) Uani 1 2 d S
F2 F 0.1094(2) 0.5000 0.0000 0.0279(7) Uani 1 2 d S
H2 H 0.0733 0.4591 -0.0006 0.034 Uiso 0.50 1 d P
Cu2 Cu 0.2500 0.26065(2) 0.2500 0.01353(15) Uani 1 2 d S
F3 F 0.41607(13) 0.26211(9) 0.25017(9) 0.0211(4) Uani 1 1 d .
H3 H 0.5000 0.264(2) 0.253(2) 0.025 Uiso 1 2 d S
N1 N 0.24902(19) 0.42707(12) 0.07561(12) 0.0161(5) Uani 1 1 d .
N2 N 0.24967(19) 0.33150(12) 0.17730(12) 0.0156(5) Uani 1 1 d .
C1 C 0.3248(2) 0.38428(15) 0.08341(15) 0.0187(6) Uani 1 1 d .
H1A H 0.3792 0.3869 0.0535 0.022 Uiso 1 1 calc R
C2 C 0.3253(2) 0.33667(15) 0.13378(15) 0.0179(6) Uani 1 1 d .
H2A H 0.3797 0.3071 0.1378 0.021 Uiso 1 1 calc R
C3 C 0.1749(2) 0.42129(15) 0.11885(15) 0.0195(6) Uani 1 1 d .
H3A H 0.1201 0.4505 0.1146 0.023 Uiso 1 1 calc R
C4 C 0.1750(2) 0.37401(15) 0.16995(15) 0.0196(6) Uani 1 1 d .
H4A H 0.1209 0.3719 0.2002 0.024 Uiso 1 1 calc R
N11 N 0.25162(19) 0.18852(12) 0.17897(12) 0.0151(5) Uani 1 1 d .
N12 N 0.2511(2) 0.08619(12) 0.08440(12) 0.0185(5) Uani 1 1 d .
C11 C 0.3277(2) 0.14721(15) 0.17258(15) 0.0196(6) Uani 1 1 d .
H11A H 0.3833 0.1524 0.2011 0.024 Uiso 1 1 calc R
C12 C 0.3268(2) 0.09671(15) 0.12484(16) 0.0210(6) Uani 1 1 d .
H12A H 0.3828 0.0685 0.1210 0.025 Uiso 1 1 calc R
C13 C 0.1737(2) 0.17885(15) 0.13860(15) 0.0194(6) Uani 1 1 d .
H13A H 0.1181 0.2074 0.1421 0.023 Uiso 1 1 calc R
C14 C 0.1741(2) 0.12760(16) 0.09201(15) 0.0203(6) Uani 1 1 d .
H14A H 0.1179 0.1215 0.0643 0.024 Uiso 1 1 calc R
Sb1 Sb 0.0000 0.003657(14) 0.207006(16) 0.01943(12) Uani 1 2 d S
Sb2 Sb 0.5000 0.207222(16) 0.999492(13) 0.02030(12) Uani 1 2 d S
F11 F 0.5000 0.11141(19) 1.00409(16) 0.0451(9) Uani 1 2 d S
F12 F 0.5000 0.20702(17) 0.90478(15) 0.0384(7) Uani 1 2 d S
F13 F 0.36207(17) 0.20779(11) 0.99911(10) 0.0355(6) Uani 1 1 d .
F14 F 0.5000 0.21611(16) 1.09406(15) 0.0363(7) Uani 1 2 d S
F15 F 0.5000 0.30228(16) 0.99572(15) 0.0341(8) Uani 1 2 d S
F21 F 0.13770(17) 0.00319(10) 0.20772(11) 0.0348(6) Uani 1 1 d .
F22 F 0.0000 0.00653(17) 0.11079(18) 0.0441(9) Uani 1 2 d S
F23 F 0.0000 0.09757(15) 0.21419(16) 0.0361(7) Uani 1 2 d S
F24 F 0.0000 -0.09049(15) 0.20896(16) 0.0378(7) Uani 1 2 d S
F25 F 0.0000 0.00078(13) 0.30242(16) 0.0313(7) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F2 Cu1 F1 180.0 . .
F2 Cu1 N1 89.87(7) . 4_565
F1 Cu1 N1 90.13(7) . 4_565
F2 Cu1 N1 89.87(7) . .
F1 Cu1 N1 90.13(7) . .
N1 Cu1 N1 179.74(14) 4_565 .
F2 Cu1 N12 89.86(6) . 16
F1 Cu1 N12 90.14(6) . 16
N1 Cu1 N12 90.20(9) 4_565 16
N1 Cu1 N12 89.80(9) . 16
F2 Cu1 N12 89.86(6) . 13
F1 Cu1 N12 90.14(6) . 13
N1 Cu1 N12 89.80(9) 4_565 13
N1 Cu1 N12 90.20(9) . 13
N12 Cu1 N12 179.72(13) 16 13
Cu1 F2 H2 121.0 . .
N11 Cu2 N11 88.88(13) . 7_545
N11 Cu2 N2 89.94(10) . .
N11 Cu2 N2 178.60(10) 7_545 .
N11 Cu2 N2 178.59(10) . 7_545
N11 Cu2 N2 89.94(10) 7_545 7_545
N2 Cu2 N2 91.25(13) . 7_545
N11 Cu2 F3 91.09(9) . 7_545
N11 Cu2 F3 89.96(9) 7_545 7_545
N2 Cu2 F3 89.29(9) . 7_545
N2 Cu2 F3 89.67(9) 7_545 7_545
N11 Cu2 F3 89.96(9) . .
N11 Cu2 F3 91.09(9) 7_545 .
N2 Cu2 F3 89.67(9) . .
N2 Cu2 F3 89.30(9) 7_545 .
F3 Cu2 F3 178.52(9) 7_545 .
Cu2 F3 H3 177(2) . .
F3 H3 F3 174(5) . 12_655
C3 N1 C1 116.7(3) . .
C3 N1 Cu1 121.8(2) . .
C1 N1 Cu1 121.5(2) . .
C4 N2 C2 117.5(3) . .
C4 N2 Cu2 121.8(2) . .
C2 N2 Cu2 120.7(2) . .
N1 C1 C2 121.6(3) . .
N1 C1 H1A 119.2 . .
C2 C1 H1A 119.2 . .
N2 C2 C1 121.0(3) . .
N2 C2 H2A 119.5 . .
C1 C2 H2A 119.5 . .
N1 C3 C4 122.2(3) . .
N1 C3 H3A 118.9 . .
C4 C3 H3A 118.9 . .
N2 C4 C3 121.0(3) . .
N2 C4 H4A 119.5 . .
C3 C4 H4A 119.5 . .
C11 N11 C13 117.8(2) . .
C11 N11 Cu2 121.3(2) . .
C13 N11 Cu2 120.9(2) . .
C12 N12 C14 116.1(3) . .
C12 N12 Cu1 122.7(2) . 13
C14 N12 Cu1 121.2(2) . 13
N11 C11 C12 120.7(3) . .
N11 C11 H11A 119.6 . .
C12 C11 H11A 119.6 . .
N12 C12 C11 122.6(3) . .
N12 C12 H12A 118.7 . .
C11 C12 H12A 118.7 . .
N11 C13 C14 120.3(3) . .
N11 C13 H13A 119.8 . .
C14 C13 H13A 119.8 . .
N12 C14 C13 122.4(3) . .
N12 C14 H14A 118.8 . .
C13 C14 H14A 118.8 . .
F21 Sb1 F21 178.96(13) 12 .
F21 Sb1 F24 89.70(6) 12 .
F21 Sb1 F24 89.70(6) . .
F21 Sb1 F23 90.25(6) 12 .
F21 Sb1 F23 90.25(6) . .
F24 Sb1 F23 174.46(16) . .
F21 Sb1 F25 89.56(7) 12 .
F21 Sb1 F25 89.56(7) . .
F24 Sb1 F25 87.08(13) . .
F23 Sb1 F25 87.38(13) . .
F21 Sb1 F22 90.44(7) 12 .
F21 Sb1 F22 90.44(7) . .
F24 Sb1 F22 92.90(14) . .
F23 Sb1 F22 92.64(14) . .
F25 Sb1 F22 179.98(13) . .
F13 Sb2 F13 179.17(14) 12_655 .
F13 Sb2 F12 89.77(6) 12_655 .
F13 Sb2 F12 89.77(6) . .
F13 Sb2 F14 90.20(6) 12_655 .
F13 Sb2 F14 90.20(6) . .
F12 Sb2 F14 174.73(16) . .
F13 Sb2 F15 89.65(7) 12_655 .
F13 Sb2 F15 89.65(7) . .
F12 Sb2 F15 87.86(13) . .
F14 Sb2 F15 86.88(13) . .
F13 Sb2 F11 90.35(7) 12_655 .
F13 Sb2 F11 90.36(7) . .
F12 Sb2 F11 92.61(14) . .
F14 Sb2 F11 92.66(14) . .
F15 Sb2 F11 179.53(13) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 F2 1.902(3) .
Cu1 F1 1.907(3) .
Cu1 N1 2.094(2) 4_565
Cu1 N1 2.094(2) .
Cu1 N12 2.405(2) 16
Cu1 N12 2.405(2) 13
F2 H2 0.9528 .
Cu2 N11 2.018(2) .
Cu2 N11 2.018(2) 7_545
Cu2 N2 2.023(2) .
Cu2 N2 2.023(2) 7_545
Cu2 F3 2.2569(18) 7_545
Cu2 F3 2.2569(18) .
F3 H3 1.142(3) .
N1 C3 1.330(4) .
N1 C1 1.347(4) .
N2 C4 1.331(4) .
N2 C2 1.347(4) .
C1 C2 1.381(4) .
C1 H1A 0.9500 .
C2 H2A 0.9500 .
C3 C4 1.388(4) .
C3 H3A 0.9500 .
C4 H4A 0.9500 .
N11 C11 1.329(4) .
N11 C13 1.343(4) .
N12 C12 1.323(4) .
N12 C14 1.342(4) .
N12 Cu1 2.405(2) 13
C11 C12 1.386(4) .
C11 H11A 0.9500 .
C12 H12A 0.9500 .
C13 C14 1.381(4) .
C13 H13A 0.9500 .
C14 H14A 0.9500 .
Sb1 F21 1.871(2) 12
Sb1 F21 1.871(2) .
Sb1 F24 1.881(3) .
Sb1 F23 1.881(3) .
Sb1 F25 1.899(3) .
Sb1 F22 1.915(4) .
Sb2 F13 1.874(2) 12_655
Sb2 F13 1.874(2) .
Sb2 F12 1.884(3) .
Sb2 F14 1.890(3) .
Sb2 F15 1.900(3) .
Sb2 F11 1.916(4) .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
F2 H2 F11 0.95 1.73 2.678(4) 175.4 13_556
